Abstract
Using MonteCarlo simulations and micromagnetic simulations, we reveal how the spin structural correlation and the skyrmion dynamics are affected by the interlayer coupling in a chiral magnetic bilayer system, in which the two layers have opposite chirality. The interaction through interlayer coupling between chiral magnetic structures influences the static and dynamics properties profoundly. The competition between the DzyaloshinskiiMoriya interaction and the interlayer interaction allows multiple magnetic structures to be energetically stable, which includes sole skyrmion states (skyrmion appears in only one of the layers) and skyrmion pair states (coupled skyrmions in top and bottom layers). When current driven spin transfer torques are applied to each state, the sole skyrmion state is mainly propelled by a spin transfer torque causing the skyrmion hall effect, but the skyrmion pair state is propelled by a torque from skyrmionskyrmion interaction and not influenced by the skyrmion hall effect. Also upon application of an external magnetic field, we found the skyrmions in a skyrmion pair state extinguish in an exclusive way, as the annihilation of a skyrmion in one of the layers stabilizes the once paired skyrmion in the other layer, i.e. the skyrmion lattice sites have only one skyrmion in either layer.
Similar content being viewed by others
Introduction
Spintronics using magnetic skyrmions has been intensively studied in recent years^{1,2,3,4,5,6,7,8,9}. Magnetic skyrmions are considered emerging candidates of a magnetic information unit due to their topological stability and good mobility. A skyrmion is topologically stable because spatially twisted magnetization provides a topological number and it cannot be destroyed or generated without a topological transition. It is also highly mobile with small spin currents since its current induced translational motion does not accompany the dissipation of energy^{10,11}. Extensive researches have been focused on manipulating the properties and dynamics of skyrmions^{12,13,14}.
Magnetic chiral structures, including skyrmions, are generated by DzyaloshinskiiMoriya(DM) interaction which twists directions of spins in an interacting spin pair^{15,16}. The scale of a chiral structure is determined by the strength of DM interaction and the chirality of the structure is determined by the direction of DM vector that is related to the symmetry of the system^{17,18}. Therefore, the strength and direction of chirality can be controlled by making an appropriate structure or interface^{19,20,21}. One of the methods to control the chirality is using interlayer coupled magnetic bilayer systems. In such systems, the coupling between the magnetic layers shows oscillatory behavior in which there can be ferromagnetic and antiferromagnetic coupling depending on the interlayer thickness. The interlayer coupling can provide an effective field which can replace an external field required to produce skyrmion structure^{22,23,24}. Also, for skyrmion pairs in antiferromagnetically coupled systems, the skyrmion Hall effect(SkHE) can be eliminated due to the cancelling skyrmion numbers of the paired skyrmions, while preserving the skyrmion properties^{25,26}.
In this study, we discuss how interlayer coupling affects the spin structure of a bilayer system in which the two layers have opposite chirality (opposite DM interaction). The opposite chirality twists the chiral structures in each layer in opposite directions, so that the DM interaction prefers to break the spin correlation between two layers. However, the interlayer coupling acts to build spin correlation against the chirality. Therefore, the competition between the DM interaction energy and the interlayer coupling energy results in complex spin structures, in which sole skyrmion states and paired skyrmion states coexist. The soleskyrmion state is a skyrmion appearing in only one of the layers, and the pairedskyrmion state is the coupled skyrmions of opposite skyrmion number in top and bottom layer. These skyrmion states are energetically stable without an external field, because the interlayer coupling provides an effective field. The dynamics of the sole skyrmion and the skyrmion pair are distinctive; When the STT in two layers are identical, the sole skyrmion is mostly influenced by the adiabatic STT and exhibit the SkHE, while the skyrmion pair is propelled by the nonadiabatic spin transfer torque(STT) without SkHE.
With an external magnetic field, skyrmion lattice composed of skyrmion pairs forms. It is composed of two skyrmions with same skyrmion number. The skyrmions in the paired skyrmion states are annihilated in a special exclusionary way, showing potential for use of these systems in spin logic circuit.
Model
We studied the bilayer system of which each layer has DM interaction of opposite chirality. The total energy of the system studied is described by the following equation;
where, S is a dimensionless and normalized vector, J the exchange constant, D_{ ij } is the DM vector, h is the external field perpendicular to the film and 1,2 indexes each layer. In our study, we set D_{1, ij} = −D_{2, ij} to implement opposite chirality and set J_{int} to be negative for the case of antiferromagnetic coupling between two layers. The cases for ferromagnetic coupling (J_{int} > 0) can be discussed by substituting S_{2}→−S_{2} in the case of h = 0.
Static magnetic structures are obtained by simulating annealing process using Monte Carlo method. Detail discussion on the simulation is described in a method section. To obtain dynamical features, we run a simulation based on LandauLifshitzGilbert equation where the effect of the STT is added;
where γ is gyromagnetic ratio, α is Gilbert damping constant. The subscript i denotes the layer number, \(u(\frac{\partial {\bf{S}}}{\partial x})\) is an adiabatic STT, and \(\beta u{\bf{S}}\times (\frac{\partial {\bf{S}}}{\partial x})\) is a nonadiabatic STT^{27,28,29}.
Results and Discussion
We first simulated two linear chain (or ladder) systems as a reduced dimensional case [Fig. 1(a)]. Without interlayer coupling, each spin chain makes a helical structure with a periodic length of 2πJ/D. When the interlayer coupling is weak (J_{int} < u_{0}), the structures of two chains are only partially correlated. The first two rows in Fig. 1(a) shows the helical structures in chain 1 and chain 2 each, and the bottom graph shows the local correlation S_{1}∙S_{2} of the spin structure. Around J_{int} ~ u_{0}, the average correlation changes abruptly indicating a phase transition. When J_{int} is just above the critical value, it still shows periodic structure, but forms the conical structure of which the net magnetization is opposite in two chains, as shown in Fig. 1(b). The correlation S_{1}∙S_{2} at J_{int} ~ u_{0} shows that small deviations from \(1\)(antiparallel) but does not vary in the full range from \({}1\) to \(1\), as shown in Fig. 1(b). The square data points in Fig. 1(c) shows how the average correlation \(\langle {{\bf{S}}}_{1}\cdot {{\bf{S}}}_{2}\rangle \) changes with J_{int}. The correlation changes abruptly around J_{int} ~ u_{0} indicating a phase transition from a helical structure to a conical structure.
The spin structure in the coupled layer system is found to be different from that of coupled spin chain system. In the coupled layer system at zero magnetic field, the spin structures obtained from Monte Carlo simulation did not show a longrange ordered structure when the system was cooled down from high temperature; skyrmions are intermixed in a complex way as in Fig. (d). This is due to the fact that interlayer coupling acts as an effective field which is required to form skyrmions in a layer system and the spins can vary spatially in any direction in the \({xy}\) plane. It indicates that multiple magnetic structures can be energetically stable. The structures shown in Fig. 1(e,f) are lattices of skyrmions, examples of the stable spin structures that appear in the coupled layer systems. These structures are obtained when we applied initial skyrmion seeds in regular arrays and released using Eq. (2). In the structure of Fig. 1(e), skyrmion pairs make a hexagonal lattice, and in the structure of Fig. 1(f), skyrmions with opposite skyrmion numbers make a square lattice. The figures show only examples of possible complex magnetic structures in which helical structures and skyrmions can coexist. In the coupled layers, the averaged correlation does not change critically at J_{int} ~ u_{0} unlike in the coupled chains [Fig. 1(c)]. However, it is not because the layered spin structures show a transitionless variation with J_{int}, but because many complex spin structures can be easily intermixed and coexist while the averaged correlation varies continuously.
As shown in Fig. 1(e,f), a skyrmion can exist as a stable state even without an external field, due to the interlayer coupling and its effective field^{30}. The effective field induced by J_{int} plays a role as a perpendicular field which stabilizes a skyrmion in the partner layer. The formation of skyrmions without any external magnetic field or anisotropy can be an advantage of this system in the spintronics applications.
We investigated the possible stable states including skyrmion. They can be classified into two cases by whether the core of a skyrmion in one layer coincides with that of other layer. Figure 2(a) shows the case where a skyrmion is in a stable state in layer 1, while layer 2 does not hold a paired skyrmion. The structure is obtained by relaxing energy from a seed structure with an initial skyrmion number, one in a layer and zero in the other layer. We refer this structure as a ‘sole skyrmion’. The spin directions in layer 2 are mostly uniform except the boundary region of the skyrmion in layer 1, therefore, the spins S_{2} in layer 2 are almost S_{2}, z ~ 1. Therefore, the effective field of interlayer coupling term can be written by \({{\bf{h}}}_{{\rm{int}}} \sim {J}_{{\rm{int}}}\hat{z}\) from Eq. (1), and this supplies a perpendicular effective field to stabilize a skyrmion in layer 1. The spin directions of layer 1 and layer 2 in the small core region of skyrmions are parallel coupled, which is against the interlayer interaction, but overall the spins follows the favored chirality in each layer. We investigated the condition to make this sole skyrmion state stable; the interlayer interaction should be in the range from stable skyrmion is from u_{0} to 4u_{0}. If J_{int} < u_{0}, an initial skyrmion becomes a helical structure, so the spatially confined round shape structure, skyrmion, is not stable. If J_{int} > 4u_{0}, a skyrmion disappears due to the strong effective field.
When a skyrmion of one layer is coupled to that of the other layer, there can be two possible states. One is that the cores of two skyrmions are spatially separated, as shown in Fig. 2(b). In this case, two sole skyrmion states are weakly coupled via inplane magnetization between two sole skyrmion states. In the state of Fig. 2(b), the core positions of two interacting skyrmions are separated, and the two skyrmions are located at a certain distance which reduces the interaction energy most. This interaction is not necessarily confined only in the two skyrmions, but generally allowed with neighboring skyrmions; therefore, interacting skyrmions make the lattice as shown in Fig. 1(f). Another is the directly coupled pair of two skyrmions which have cores at the same position as in Fig. 2(c). This direct type of skyrmion pairs builds the lattice structure as shown in Fig. 1(e). We refer it as a ‘skyrmion pair’. In this case, core area is wider than a sole skyrmion and has a thin inplane part which is partially chiral. The inplane part has tilted magnetism carrying both Blochtype magnetization due to the interlayer interaction and the chiral Néeltype magnetization due to the DM interaction. Therefore, this structure is neither a Néel nor a Bloch type skyrmion. Though a sole skyrmion becomes unstable if J_{int} > 4u_{0}, because the effective fields from other layer becomes too strong, the skyrmion pair is still stable in the range of J_{int} > 4u_{0}, since their cores are also coupled by interlayer interaction and the effective fields supports the core magnetization. Therefore, in the range of J_{int} > 4u_{0}, only the skyrmion pair state is energetically stable and the sole skyrmion state is not. In the range of u_{0} < J_{int} < 4u_{0}, the structures in Fig. 2(b,c) are both energetically stable, hence both exist together and are mixed resulting in complex magnetic structures such as those shown in Fig. 1(d).
The dynamics of a skyrmion pair and a sole skyrmion under a STT is very different from each other. It is known that the skyrmion pair can move directly along the current direction without SkHE, because the skyrmion number is canceled by the sum of two skyrmion numbers. Here, we find that additionally, the motion of a sole skyrmion and the motion of a skyrmion pair have distinctive characteristics, depending on whether the motion is caused by adiabatic or nonadiabatic STT. To clearly show the difference between adiabatic and nonadiabatic STTs, we only applied one of them in the simulation introducing an additional velocity term ν(=uβ/α) related to the nonadiabatic torque. Therefore, the portion of u and v estimates the contribution of the adiabatic and the nonadiabatic STT in skyrmion dynamic, respectively. The adiabatic STT contributing to the spin dynamics is \(u(\frac{\partial {\bf{S}}}{\partial x})\) and the nonadiabatic STT contribution is \(\alpha v{\bf{S}}\times (\frac{\partial {\bf{S}}}{\partial x})\).
Figure 3(a) compares the dynamics of a sole skyrmion and skyrmion pair under identical adiabatic STTs in each layer (u_{1} = u_{2} = u, ν_{1} = ν_{2} = 0). Under the adiabatic STT, a sole skyrmion moves in a diagonal direction to the current direction u showing the SkHE. The SkHE of the sole skyrmion in layer 1 (left panel in Fig. 3(a)) and the SkHE of the sole skyrmion in layer 2 (middle panel in Fig. 3(a)) is opposite since the skyrmions have opposite chirality. In the case of two sole skyrmion state weakly coupled by inplane edges (Fig. 2(b)), each skyrmion is found to follow the dynamic of a sole skyrmion and soon be separated, not affected much from other skyrmion. Though two skyrmions are coupled via inplane magnetization, this coupling was not strong enough to cause different dynamic.
However, the skyrmion pair (Fig. 2(c)) showed very different dynamics; it stays still, not moving at all under the same condition, so we can see that the adiabatic STT cannot activate a motion of the skyrmion pair. The skyrmion in each layer has a skyrmion number of opposite sign. Therefore, the forces produced by the adiabatic STT [Red arrows in figures] are opposite and the directions of SkHE are opposite as well. For interlayer coupling strong enough to bound the two skyrmions, the force induced by the J_{int} is opposite to the SkHE direction. It attracts the partner skyrmion to prevent the increase of the interlayer interaction energy [blue arrows in Fig. 3(a)]. As the forces from J_{int} and adiabatic STT are opposite, they act against to each other and the net force on a skyrmion is canceled out.
The motions under the identical nonadiabatic STTs (u_{1} = u_{2} = 0, ν_{1} = ν_{2} = ν) in each layer are represented in Fig. 3(b). In this case, a sole skyrmion shows motion nearly perpendicular to the current direction; however, the magnitude of the displacement is much smaller compared to the adiabatic STT induced motion and the tilting direction is opposite to the direction of the adiabatic STT case. The directions of SkHE induced by the nonadiabatic STT of each layer are also opposite due to the different sign of the skyrmion number, but the forces ακ∙ν from nonadiabatic STT are in the same direction[Green arrows in Fig. 3(b)].
On the other hand, The skyrmion pair drifts along the direction of v, faster than the sole skyrmion. In this case, interlayer interaction also provides an attractive force to prevent the decoupling of skyrmion pair. Since the force from J_{int} is perpendicular to the force from the nonadiabatic STT, it is not canceled out and produces a nonzero torque. Though the directions of forces on two skyrmions are opposite to each other, the gyrodynamic motion propels each skyrmion in the same direction because of their opposite skyrmion number. It needs to be noted that the torques propelling skyrmions are not the STT but the attraction force binding two skyrmions against SkHE. Therefore, the gyrodynamic motion produces a fast drift, even though the force from STT is not strong. And the drift motion is perpendicular to the motion caused by SkHE that is perpendicular to the current direction, therefore, the skyrmion pair moves along the current direction.
In the case when the both STTs equally contribute (u = ν) [Fig. 3(c)], The motions of a sole skyrmion and a skyrmion pair become similar to each other.
We compared our simulation results with the analysis with Thiele equation^{31,32,33} which is a standard tool to analyses the skyrmion or vortex motion, especially, for the paired skyrmion or vortices under the action of STT effect. The Thiele equations for the skyrmions under STT are
where \(\dot{{\bf{r}}}\) is the drift velocity of skyrmion, α is the Gilbert damping constant, and V_{ ij } is the potential induced by the other layer. G_{ i } and κ_{ i } are gyromagnetic coupling vector and dissipative dyadic tensor of the magnetic structure each layer. The directions of u_{i} and v_{i} are xdirection. The gyromagnetic coupling vectors and the dissipative dyadic tensors are related to the topological properties of the magnetic structure and their magnitudes are \({\rm{G}}=\int {\bf{S}}\cdot ({\partial }_{x}{\bf{S}}\times {\partial }_{y}{\bf{S}})\) and \(\kappa =\int {\partial }_{x}{\bf{S}}\cdot {\partial }_{x}{\bf{S}}\cong \int {\partial }_{y}{\bf{S}}\cdot {\partial }_{y}{\bf{S}}\).
For the case of a sole skyrmion, G_{1} = G, κ_{1} + κ_{2} = κ_{tot} and the solution is
The equation can be approximated as \({\dot{x}}_{1}={u}_{1}\) and \({\dot{y}}_{1}=0\) especially when α is small (\(\alpha < < \frac{{\rm{G}}}{\kappa }\)). From the equations, we can see that the motion of a sole skyrmion is mostly dependent on the adiabatic STT. If a skyrmion is in layer 1 only, the STT on layer 2 has little influence on its motion. The motions along \(\hat{x}\) caused by u and ν are same along the current direction, but the motion along \(\hat{y}\) by SkHE is opposite for u and ν. It is important because the direction of the interaction force −∇V induced by the interlayer interaction is opposite to the direction of the force separating the coupled skyrmion induced by the current and the produced torques from the interaction forces are opposite as well.
In a strongly coupled skyrmion pair in a weak current, the spins in pair sites are all opposite and move together (r_{1} = r_{2}); thus, G_{1} = −G_{2} = G, κ_{1} = κ_{2} and the interaction between two skyrmion acts to the opposite direction ∇V_{12} = −∇V_{21}. Therefore, the total gyromagnetic coupling vector G_{tot} is zero and total dyadic tensor κ_{tot} is 2κ_{1} (or 2κ_{2}). When two skyrmions are strongly coupled and move together, the drift velocity of a strongly coupled skyrmion pair is
The interaction force acting on a skyrmion of layer 1 in the skyrmion pair is
If the STT in layer 1 and 2 are identical(u_{1} = u_{2} = u and ν_{1} = ν_{2} = ν), The force along the current direction is zero (F_{x,1} = −F_{x,2} = 0) and the force along the current direction is F_{y,1} = −F_{y,2} = G(ν−u). Therefore, the forces from the adiabatic STT and the nonadiabatic STT have opposite direction to each other. When the skyrmions of each layer are under STTs, the SkHE along ydirection makes both skyrmions separate from each other. The interlayer interaction, however, is strong enough to maintain the skyrmion pair, hence the origin of the force in Eq. (6) is the restoring force to overcome opposite gyrodynamic motion caused by the opposite skyrmion number.
Since the equation of motion is \({\rm{G}}{\dot{x}}_{1}={\rm{G}}{u}_{1}\frac{\partial V}{\partial {y}_{1}}\alpha {\kappa }_{1}{\dot{y}}_{1}={\rm{G}}u+G(vu)0={\rm{G}}v\), the interaction force caused by the adiabatic STT, −Gu is canceled out with the direct force from adiabatic STT, Gu. Therefore, the net force on skyrmion pair caused by the adiabatic STT is zero and the motion along the current direction is only affected by the interaction force −Gν which is originated from nonadiabatic STT. As a result, the propelling torques for a skyrmion pair and a sole skyrmion is distinctive. The former is nonadiabatic STT, and the latter is adiabatic STT.
If the STT in two layers are not identical, the motion can be described by Eq. 6 in general. Especially when the STTs are exactly opposite to each other (u_{1} = −u_{2} and ν_{1} = −ν_{2}), only F_{ x } contributes and skyrmion pair moves in the y direction. In this case, the propelling torque for a skyrmion pair becomes the adiabatic STT.
The dynamics of a skyrmion is influenced by pinning potentials, though it is robust and less affected by impurities or nonadiabatic effect than other magnetic structures^{34,35,36}. Although a skyrmion pair moves only with nonadiabatic STT, it is not because of the direct effect from nonadiabatic STT, but because of the attractive interaction between the two skyrmions. Hence, the dynamics of the skyrmion pair is influenced by impurities as much as a single skyrmion is. Since the total gyromagnetic coupling vector, G, of a skyrmion pair is zero, the detailed dynamics from a pinning potential is different: a skyrmion pair moves straight while a sole skyrmion moves spirally around the attraction center (Fig. 4).
When an external field h ~ u_{0} is applied, the paired (coupled) skyrmion lattice structure can be stabilized (Fig. 5). Note that the skyrmion pair is not the same kind of skyrmion pair in Fig. 2. Under external field(h ~ J_{int}), skyrmions composing a pair with the same skyrmion number, because the magnetic field overcome the interlayer interaction and the skyrmions have same magnetic background (shown as white color in figure). The simulation results show that the spins in the core region of the paired skyrmions are parallel but the spins in the rim of a skyrmion in layer 1 is antiferromagnetically coupled with that of the skyrmion in layer 2 to reduce the J_{int} energy. Therefore, the skyrmions in two layers have the same polarity but opposite chirality. As J_{int} is increased, the area of the rim (or boundary) region of the coupled skyrmion, which have opposite inplane magnetizations in the top and bottom layers, increases to reduce the interlayer coupling energy. Therefore, the size of skyrmions increases with J_{int} accordingly (Fig. 5). When the interlayer coupling is weak (J_{int} < u_{0}) or moderate (J_{int} ~ u_{0}), skyrmions form a coupled hexagonal lattice with matching skyrmion lattice sites in the top and bottom layers [Fig. 5(a,b)]. The skyrmions in the top and bottom layers have opposite chirality with the inplane boundary regions having opposite magnetization and the core regions having the same polarity. When J_{int} is strong (J_{int}>>u_{0}), skyrmion shape becomes irregular and the longrange order forming lattice structure is reduced [Fig. 2(c)]. The strong J_{int} increases area of the rim (or boundary) of skyrmions where the spin profile is flattened, thus the role of DM interaction causing regular chiral structure is reduced.
As the external field is increased, some of the skyrmions are annihilated. The series of figures [Fig. 6(a–c)] shows how the skyrmions are extinguished. Since two layers are identical (J_{1} = J_{2} and D_{1} = D_{2}), the annihilation process is random: skyrmions in top layers are extinguished at some lattice sites while skyrmions in the bottom layer are extinguished in other lattice site. In Fig. 6(a), the behavior is somewhat exclusive at this stage, so a skyrmions in one layer is extinguished while the skyrmion in other layer is preserved. As one skyrmion of the coupled skyrmion is annihilated, another skyrmion gets to occupy more area and the regularity of the hexagonal order is broken [Fig. 6(a)]. The extinguishment of the skyrmion in one layer reduces the frustration caused by antiferromagnetic interlayer interaction and stabilizes the now unpaired skyrmion in the other layer. This results in the remaining skyrmion being stabilized and becoming larger. At a certain external field (Fig. 6(b)), every skyrmion lattice site has only one skyrmion either in the layer 1 or the layer 2. A regular hexagonal structure is rebuilt if both layers are combined, though the skyrmions in each layer do not make a regular structure. Since one skyrmion lattice site can be considered as one bit of memory/information, this exclusive nature can be potentially useful for spin logic operation such as ‘inverse’ or ‘exclusive or’, especially when considering the fact that the information of two near lattice sites within a layer does not interfere with each other. When the magnetic field if further increased, the remaining skyrmion become extinguished as well and the hexagonal order through both layers is broken again [Fig. 6(c)].
Conclusion
We investigated the skyrmion structures and their dynamics in interlayer coupled systems when the chirality are opposite in two layers. Skyrmions and skyrmion pairs are stable state without an external field. A skyrmion pair exhibits different dynamics from a sole skyrmion without pairing another skyrmion in the other layer. When the STT in two layers are identical, the former is propelled by skyrmionskyrmion interaction and moves along the spin current, while the latter is mostly propelled by adiabatic STT and moves in the oblique direction. Under an external field, skyrmions in the skyrmion lattice disappear in an exclusive way in which a skyrmion in one layer is extinguished prior to that of another layer during the magnetic saturation process.
Methods
In simulation, we used square spin grids composed of ~10^{6} spins interacting with neighborhood four spins via exchange interaction and DMI (Eq. 1). We did not consider magnetic anisotropy or magnetic dipole interaction, and the parameters of each layer were set to be identical except the sign of the DM interaction in order to simplify the scopes of our study. The antiferromagnetic interlayer coupling case is studied; however, generalization to the ferromagnetic case can be done by substituting S_{2}→−S_{2} in the case of h = 0. The direction of a DM vector is set to perpendicular to r_{ij}^{37,38}, but can also be generalized to the parallel case(D_{ij}r_{ij})^{39,40} by S_{ x }→S_{ y }, S_{ y }→−S_{ x }, where r_{ij} is the displacement vector between i and j spins. Therefore, some of our results and discussion are valid for ferromagnetic interlayer coupling case and other types of DM interaction. However, it should be noted that the case of an opposite chirality cannot be converted to the case of an identical chirality by such a simple symmetry operation.
When only a layer with J and D is considered, the periodic length of a chiral structure is proportional to J/D and the effective field from DM interaction to form chiral structure such as a skyrmion lattice is proportional to D^{2}/J^{19}. Therefore, we use J/D to discuss the periodic length of the chiral structure and D^{2}/J to discuss the strengths of effective fields. In our simulation, we typically used J = 1 and D = 0.2, however, the values do not affect results after we convert length and field units to L_{0} = 2πJ/D and u_{0} = D^{2}/J as long as D<<J. In the continuum approximation, the energy density unit becomes \({u}_{0}=\frac{{{D}_{M}}^{2}}{2A}\) and length unit becomes \({L}_{0}=4\pi \frac{A}{{D}_{M}}\), where A is the exchange stiffness and D_{ M } is the DMI strength. The real parameters for typical DM system are listed by L_{ D } = L_{0}, related to the periodic length of chiral structure, and h_{ D } = Mu_{0}, related to the required field strength to form skyrmion lattice. Here, a is a lattice constant, and M is the magnetization vector^{41}. As an example, L_{ D } and h_{ D } of FeGe are 70 nm and 0.4 T.
To investigate the magnetic ground state or stable state, we run Monte Carlo simulations based on a heat bath method^{42}. In the method, a temperature parameter was slowly decreased maintaining the thermally stable state at specific external field strength, until we obtain a stable state which does not vary with further iterations any more. In the stable states, every spin is along its local effective field \({{\bf{H}}}_{i,\mathrm{eff}}={\partial U/\partial {\bf{S}}}_{{\rm{i}}}\). To make structures with definite skyrmion numbers (Fig. 1(e,f) and Fig. 2), we started the simulation from initial structures having skyrmion numbers same as the final stable structures. To investigate the dynamic feature of skyrmion such as the motion under spin transfer torques, we numerically solved LLG equation (Eq. 2) and the motions obtained from the simulation are compared with the analytic solution from the Thiele equation(Eq. 3).
References
Nagaosa, N. & Tokura, Y. Topological properties and dynamics of magnetic skyrmions. Nat. Nanotechnol. 8(12), 899–911 (2013).
Woo, S. et al. Observation of room temperature magnetic skyrmions and their currentdriven dynamics in ultrathin Co films. arXiv preprint arXiv: 1502.07376 (2016).
Iwasaki, J. et al. Currentinduced skyrmion dynamics in constricted geometries. Nat. Nanotechnol. 8(10), 742–747 (2013).
Yu, X. Z. et al. Skyrmion flow near room temperature in an ultralow current density. Nat. Commun. 3, 988 (2012).
Fert, A., Cros, V. & Sampaio, J. Skyrmions on the track. Nature nanotechnology. Nat. Nanotechnol. 8(3), 152–156 (2013).
Wiesendanger, R. Nanoscale magnetic skyrmions in metallic films and multilayers: a new twist for spintronics. Nat. Rev. Mat. 1, 16044 (2016).
Legrand, W. et al. Roomtemperature currentinduced generation and motion of sub100 nm skyrmions. Nano Lett. 17(4), 2703–2712 (2017).
Krause, S. & Wiesendanger, R. Spintronics: Skyrmionics gets hot. Nat. Mat. 15(5), 493–494 (2016).
Rosch, A. Spintronics: Electric control of skyrmions. Nat. Nanotechnol. 12, 103–104 (2016).
Jonietz, F. et al. Spin transfer torques in MnSi at ultralow current densities. Science 330(6011), 1648–1651 (2010).
Iwasaki, J., Koshibae, W. & Nagaosa, N. Colossal spin transfer torque effect on skyrmion along the edge. Nano Lett. 14(8), 4432–4437 (2014).
Dupé, B., Bihlmayer, G., Böttcher, M., Blügel, S. & Heinze, S. Engineering skyrmions in transitionmetal multilayers for spintronics. Nat. Commun. 7, 11779 (2016).
Zhang, X. et al. Control and manipulation of a magnetic skyrmionium in nanostructures. Phys. Rev. B 94(9), 94420 (2016).
Wang, Z. & Grimson, M. J. Driving skyrmions in a composite bilayer. Phys. Rev. B 94(1), 14311 (2016).
Dzyaloshinsky, I. A thermodynamic theory of “weak” ferromagnetism of antiferromagnetics. J. Phys. and Chem. of Solids 4(4), 241–255 (1958).
Moriya, T. Anisotropic superexchange interaction and weak ferromagnetism. Phys. Rev. 120(1), 91 (1960).
Kwon, H. Y., Bu, K. M., Wu, Y. Z. & Won, C. Effect of anisotropy and dipole interaction on longrange order magnetic structures generated by Dzyaloshinskii–Moriya interaction. J. Mag. and Mag. Mat. 324(13), 2171–2176 (2012).
Kwon, H. Y. & Won, C. Effects of Dzyaloshinskii–Moriya interaction on magnetic stripe domains. J. Mag. and Mag. Mat. 351, 8–15 (2014).
Chen, G. et al. Tailoring the chirality of magnetic domain walls by interface engineering. Nature communications. Nat. Commun. 4, 2671 (2013).
Chen, G. et al. Unlocking Blochtype chirality in ultrathin magnets through uniaxial strain. Nat. Commun. 6, 6598 (2015).
Chen, G. et al. Outofplane chiral domain wall spinstructures in ultrathin inplane magnets. Nat. Commun. 8, 15302 (2017).
Kang, S. P., Kwon, H. Y., Kim, H. S., Shim, J. H. & Won, C. Effect of interlayer exchange coupling on magnetic chiral structures. J. App. Phys. 118(4), 43905 (2015).
Nandy, A. K., Kiselev, N. S. & Blügel, S. Interlayer exchange coupling: a general scheme turning chiral magnets into magnetic multilayers carrying atomicscale skyrmions. Phys. Rev. Lett. 116(17), 177202 (2016).
Chen, G., Mascaraque, A., N’Diaye, A. T. & Schmid, A. K. Room temperature skyrmion ground state stabilized through interlayer exchange coupling. App. Phys. Lett. 106(24), 242404 (2015).
Zhang, X., Zhou, Y. & Ezawa, M. Magnetic bilayerskyrmions without skyrmion Hall effect. Nat. Commun. 7, 10293 (2016).
Koshibae, W. & Nagaosa, N. Theory of skyrmions in bilayer systems. Scientific Reports, Sci. Reports 7, 42645 (2017).
Thiaville, A., Rohart, S., Jué, É., Cros, V. & Fert, A. Dynamics of Dzyaloshinskii domain walls in ultrathin magnetic films. Europhysics Lett. 100(5), 57002 (2012).
Thiaville, A., Nakatani, Y., Miltat, J. & Suzuki, Y. Micromagnetic understanding of currentdriven domain wall motion in patterned nanowires. Europhysics Lett. 69(6), 990 (2005).
Hals, K. M. & Brataas, A. Spintransfer torques in helimagnets. Phys. Rev. B 87(17), 174409 (2013).
Bogdanov, A. & Hubert, A. Thermodynamically stable magnetic vortex states in magnetic crystals. J. Mag. and Mag. Mat. 138(3), 255–269 (1994).
Thiele, A. A. Steadystate motion of magnetic domains. Phys. Rev. Lett. 30(6), 230 (1973).
Liu, Y., Hou, Z., Gliga, S. & Hertel, R. Influence of the dynamic dipolar interaction on the currentinduced core switch in vortex pairs. Phys. Rev. B 79(10), 104435 (2009).
He, J., Li, Z. & Zhang, S. Currentdriven vortex domain wall dynamics by micromagnetic simulations. Phys. Rev. B 73(18), 184408 (2006).
Iwasaki, J., Mochizuki, M. & Nagaosa, N. Universal currentvelocity relation of skyrmion motion in chiral magnets. Nat. Commun. 4, 1463 (2013).
Martinez, J. C. & Jalil, M. B. A. Topological dynamics and currentinduced motion in a skyrmion lattice. New J. Phys. 18(3), 033008 (2016).
Liu, Y. H. & Li, Y. Q. A mechanism to pin skyrmions in chiral magnets. J. Phys.: Condens. Matter 25(7), 076005 (2013).
Deák, A., Szunyogh, L. & Ujfalussy, B. Thicknessdependent magnetic structure of ultrathin Fe/Ir (001) films: From spinspiral states toward ferromagnetic order. Phys. Rev. B 84(22), 224413 (2011).
Bode, M. et al. Chiral magnetic order at surfaces driven by inversion asymmetry. Nature 447(7141), 190–193 (2007).
Mühlbauer, S. et al. Skyrmion lattice in a chiral magnet. Science 323(5916), 915–919 (2009).
Shibata, K. et al. Towards control of the size and helicity of skyrmions in helimagnetic alloys by spinorbit coupling. Nat. Nanotechnol. 8(10), 723–738 (2013).
Wilhelm, H. et al. Confinement of chiral magnetic modulations in the precursor region of FeGe. J. Phys.: Condens. Matter 24(29), 294204 (2012).
Kwon, H. Y. et al. A study of the stripe domain phase at the spin reorientation transition of twodimensional magnetic system. J. Mag. and Mag. Mat. 322(18), 2742–2748 (2010).
Acknowledgements
This research was supported by the National Research Foundation of Korea funded by the Korean Government (Grant No. 2015R1D1A1A01056971), by the National Research Council of Science and Technology (NST) grant (No. CAP1601KIST) by the Korea government, and the KIST Institutional Program (2E27140).
Author information
Authors and Affiliations
Contributions
S.P.Kang, J.W.Choi, B.C.Min and C.Won designed the model and methods. S.P.Kang. N.J.Kim and H.Y.Kwon performed the computer simulation, C.Won, S.P.Kang analyzed the results, and all the coauthors participated the discussion on the results. S.P.Kang and C.Won wrote the paper and all the coauthors commented on it.
Corresponding author
Ethics declarations
Competing Interests
The authors declare that they have no competing interests.
Additional information
Publisher's note: Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Rights and permissions
Open Access This article is licensed under a Creative Commons Attribution 4.0 International License, which permits use, sharing, adaptation, distribution and reproduction in any medium or format, as long as you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in a credit line to the material. If material is not included in the article’s Creative Commons license and your intended use is not permitted by statutory regulation or exceeds the permitted use, you will need to obtain permission directly from the copyright holder. To view a copy of this license, visit http://creativecommons.org/licenses/by/4.0/.
About this article
Cite this article
Kang, S.P., Kim, N.J., Kwon, H.Y. et al. The spin structures of interlayer coupled magnetic films with opposite chirality. Sci Rep 8, 2361 (2018). https://doi.org/10.1038/s41598018208008
Received:
Accepted:
Published:
DOI: https://doi.org/10.1038/s41598018208008
This article is cited by

Direct currenttunable MHz to multiGHz skyrmion generation and control
Scientific Reports (2019)

Symmetrybreaking interlayer Dzyaloshinskii–Moriya interactions in synthetic antiferromagnets
Nature Materials (2019)
Comments
By submitting a comment you agree to abide by our Terms and Community Guidelines. If you find something abusive or that does not comply with our terms or guidelines please flag it as inappropriate.